# ENGN2340 â€“ Final Project Computational rate Tzoumaka Fall 2017 ENGN2340...

date post

21-May-2018Category

## Documents

view

216download

2

Embed Size (px)

### Transcript of ENGN2340 â€“ Final Project Computational rate Tzoumaka Fall 2017 ENGN2340...

Anastasia Tzoumaka

Fall 2017

ENGN2340 Final Project

Computational rate independent Single Crystal Plasticity with

finite deformations Abaqus Umat Implementation

Intorduction:

Single crystals, are monocrystalline solids whose structure consists of a single, continuous and

unbroken grain. They are characterized by their extraordinary mechanical properties,

which are mainly attributed to the absence of structural defects associated with grain boundaries.

These properties and especially the inherent creep resistance of metal single crystals is the main

reason for their widespread implementation in turbines and the energy industry. However, research

on the mechanical behavior and constitutive modelling of single crystals is not entirely motivated by

the continuous need for innovative industrial applications. Each and every metal consists of grains

and grain boundaries and all metals share the same defects such as vacancies, dislocations etc. Single

crystals are essentially the building block of every polycrystalline metal that existed, exist and will

exist in the future since by definition, single crystals only consist of a single grain with a given spatial

orientation and no boundaries. Understanding the mechanics of crystal plasticity and being able to

simulate the deformation of single crystals is therefore crucial to the understanding of very important

phenomena in metals such as texture, deformation induced anisotropy, grain interactions and many

more. In this project we will focus on FCC crystals since they represent the vast majority of metals

used in engineering applications. We will present the fundamental theory behind single crystal

plasticity, outline the governing equations and describe the methods that can be used to solve the

equations numerically in a finite element setting. The constitutive model will then be implemented

in a User MATerial subroutine that can be used with the Abaqus commercial FEA software and the

code will be tested in a series of simulations designed to assess the convergence and validity of the

results.

Elastoplastic equations:

The physically based assumption, that crystal plasticity is the result of simultaneous simple shears

along the crystal's active systems allows us to express the velocity gradient associated with plastic

slip as (Bower):

where 0 0,s m

are the unit vectors along the slip and normal directions of slip system respectively,

defined in the reference configuration 0 . The summation in the above equations is carried over

the active systems at the time of calculation Nas (Number of Active Systems). Now recalling that the

deformation rate D and spin tensor W are defined as the symmetric and skew parts of L respectively,

we can also define:

The multiplicative decomposition of the deformation gradient F :

The slip direction vector 0s

is embedded in the lattice and transforms during deformation according

to 0es s F . In contrast, the unit normal to the slip plane

0m transforms as 0

em m F , so that

it constantly remains perpendicular to the slip plane.

The Elasticicty Matrix:

The constitutive relationship for the elastic behavior of an FCC metal single crystal is taken to be

that of an linearly elastic solid with cubic symmetry. In this case the constitutive law can be

parameterized with respect to 3 independent material constants and with respect to the crystal axes

can be written in the form (Bower):

Where:

Is the elasticicty matrix with respect to the crystal axes and in terms of ijC .

Finally:

Hardening of Single Crystal: The Bassani-Wu Model

A typical stress--strain curve of an FCC metal crystal exhibits three distinct deformation stages

(Haidemenopoulos ). Initially, in Stage I, plastic slip is attributed to the activation of only one out of

the twelve possible slip systems that FCC crystals comprise of 12 slip systems resulting from all

possible combinations between their 4 dense planes and 3 dense directions

The yield criterion of each slip system is defined in terms of the resolved shear stresses and is expressed in rate form as:

The consistency condition then takes the following form for every slip system a:

The hardening model proposed by Bassani and Wu is then summarized as:

Rate Independent Tangent Modulus

Elasticicty:

Plasticity:

Where:

1[ ]

UMAT implementation Stress Update Algorithms :

The resolved shear stress within each slip system a can be calculated as:

The hardening of each slip system is then expressed as:

The yie ld conditions of all slip systems are then introduced in terms of the two above equations:

Therefore, the unknowns are determined as the solution of the following system:

Only numerical solutions are applicable to the above equation since both and cr are highly non-

-linear functions of the unknowns . Implementing the Newton Raphson method, we can

iteratively solve for the unknowns until convergence is achieved. Newton iterations for

multivariate systems however, require the Jacobian matrix of the system, which in this case is defined

as ( / )a . Next, we calculate the derivatives necessary to build the Jacobian matrix:

Variation of eF with respect to :

Right Cauchy-Green elastic tensor variation:

Green strain variation:

2nd Piolla Kirchhoffs variation:

Calculating the derivative ( / )

Variation of the resolved shear stress on a system with respect to all slips

Criticla shear stress variation :

Final expression of the elastic Jacobian

Figure 4: Schematic representation of the stress update algorithm

Results :

Figure 5 illustrates the anisotropic and non-uniform deformation of the sinlg crystal specimen

presenting the actual undeformed and deformed shapes before and after the uniaxial analysis.

Figure 5: Undeformed and deformed configuration

The finite element results for the uniaxial tension are presented in figure 6 by plotting the

macroscopic true stress-logarithmic strain curve.

Figure 6: Stress - logarithmic strain curve for uniaxial tension

In total, 11 slip systems are activated during the uniaxial tension test, and the order of activation is

in complete agreement with the one predicted using the Schmid factors:

Slip System Schmid Factor

5 0.489897949 2 0.419912527 6 -0.326598632 7 -0.279941685

1,3 -0.209956264 4 -0.163299316

8,9 0.139970842 10 -0.093313895 11 0.069985421 12 0.023328474

*View more*